Biogenic Metal Oxides

Biogenic metal oxides (MxOy) feature structures as highly functional and unique as the organisms generating them. They have caught the attention of scientists for the development of novel materials by biomimicry. In order to understand how biogenic MxOy could inspire novel technologies, we have reviewed examples of all biogenic MxOy, as well as the current state of understanding of the interactions between the inorganic MxOy and the biological matter they originate from and are connected to. In this review, we first summarize the origins of the precursors that living nature converts into MxOy. From the point-of-view of our materials chemists, we present an overview of the biogenesis of silica, iron and manganese oxides, as the only reported biogenic MxOy to date. These MxOy are found across all five kingdoms (bacteria, protoctista, fungi, plants and animals). We discuss the key molecules involved in the biosynthesis of MxOy, the functionality of the MxOy structures, and the techniques by which the biogenic MxOy can be studied. We close by outlining the biomimetic approaches inspired by biogenic MxOy materials and their challenges, and we point at promising directions for future organic-inorganic materials and their synthesis.


Introduction
Living organisms-from bacteria to plants and mammals-have developed functional materials to optimize their life. Functions that materials in living beings provide are, e.g., mechanical support and protection, light-harvesting (e.g., for photosynthesis), and navigation. While living beings are for the largest part composed of organic matter, quite a range of functional materials in living beings are of inorganic nature and recognized as of biogenic origin. The term 'biogenic', from Greek bíos (life) + génos (origin), means produced by living organisms. For instance, both certain bacteria, and bees use magnetic iron oxide particles as part of their navigation systems [1,2]. Another example are silica (SiO 2 ) structures that are manufactured by diatoms, marine sponges, and plants, for protection of the organism [3]. The two latter examples of inorganic materials in living beings, Fe 3 O 4 and SiO 2 , are both biogenic metal oxides. Aside from metal oxides, one finds other inorganic compounds in living beings. Yet, the overall number of biogenic inorganic compounds is very limited. To date, not more than a few dozens of inorganic materials have been identified in living beings [4]. The main inorganic materials found in organisms are metal carbonates, phosphates, halides, oxalates, sulfates, sulfides, and oxides [5]. Nearly all of these compounds belong to the realm of minerals, which are defined as being (i) crystalline, (ii) inorganic, and (iii) naturally occurring materials. When minerals are occurring as part of living beings, they are named 'biominerals'. Minerals that are part of living beings are very much affected by their environment, e.g., the presence of biomolecules such as proteins and sugars affect crystallite sizes and shapes, which in turn has drastic effects on the final materials properties. The term 'biominerals' nicely differentiates them from minerals the different mineralizing species, as a species that would limit itself to scarce elements would not have the best chances of survival. Second, the latter compounds are typically highly water-insoluble. As living beings are water-based or even live in aqueous environments such as oceans, it is necessary that their protective shell or stability-giving skeleton does not dissolve in water. Additionally, the low water-solubility imparts the final biominerals to nucleate at high supersaturation, which eventually promotes the formation of many small crystallites. Small, mostly nano-sized, crystallites are in living beings often found in well-organized nanocomposites that, e.g., mechanically profit from the small crystallite sizes, and also allow for generating complex shapes even including curvature. Third, while the inorganic parts of many biominerals are typically highly water insoluble, they often exist as hydroxylated/hydrated intermediates [8]. The existence of such water-soluble intermediates is necessary so that the organisms can actually manipulate these precursors before they deposit the final biominerals at the desired place within the organism. Finally, both the involved ions can be nicely manipulated through living beings, which have a machinery (e.g., calcium-ion channels) that is well adapted to work with these species.
With this review, we give an overview of metal oxides (M x O y ) found in living systems (note that while in many review articles metal oxides are often abbreviated as 'MO', we decided to herein use M x O y to avoid confusion with 'MO' as common abbreviation of 'molecular orbital'). Metal oxides are of particular interest in materials chemistry as, (i) they are useful for various applications, e.g., as magnetic materials, catalysts, or optical materials; and (ii) they can be synthesized by molecular bottom-up approaches (mostly notably through the sol-gel process). Important M x O y are, for example, TiO 2 (a powerful photocatalyst), Fe 3 O 4 (a biocompatible magnetic material), and CeO 2 (an important oxidative catalyst) [9]. The applications of M x O y are significantly different to salt-type components in biominerals such as CaCO 3 , which are important components for, e.g., biomedical applications or construction. Structurally, the metal oxides found in living organisms are actually built up of covalent and/or iono-covalent bonds, which again is fundamentally different from salt-type biominerals. As (living) nature is one of the best sources of inspiration, we hope that reviewing metal oxides in living organisms might be of interest to materials scientists, chemists, physicists, and engineers, that are rather far away from biology. To enable an easy entry point for this broad range of disciplines, we have assumed a rather tutorial writing style. For allowing for accessibility of this review to chemists, materials and physicists scientists, we have taken case to explain the biological technical terms in footnotes. As material chemists, at the end of this review we are providing a perspective for materials chemistry.
While biominerals have been widely reviewed focusing on particular aspects, e.g., specific chemical or biological compositions [1,[10][11][12][13]; evolutionary aspects [7]; organic-inorganic interfaces [14]; or with respect to some particular technological applications, such as the production of inorganic materials (e.g., ceramic oxides, semiconductors and metal nanoparticles) [15], we are not aware of any other review that exclusively focuses on metal oxides found in living systems and therefore hope to close this gap.

Origins of the Precursors of Biogenic Metal Oxides
The Earth's crust consists primarily (~90%) of silicates, i.e., minerals built up of anions of silicon and oxygen (i.e., [SiO 4 − 2 4 − -]n in, e.g., orthosilicate SiO4 4− , metasilicate SiO3 2− , and pyrosilicate Si2O7 6− ). Metal cations (e.g., Fe 2+ , Mn 2+ , Al 3+ and Si 4+ ) can be released from silicates by weathering (Figure 2A-C). Weathering describes the breakdown of igneous, metamorphic and sedimentary rocks, through the action of water, temperature and biological activity. The mechanical, microbiological as well as chemical weathering lead the transformation of mineral rocks to so-called mineral soil. The minerals present in the soil are chemically altered in this process (see reactions I-III in Figure 2), releasing water-soluble ions into their surroundings. Through water circulation in and above ground, these species are transported to different loci and later are taken up by living organisms (for instance, through the roots of plants) as we will see later.
The three biogenic metal oxides are SiO2, FexOy (e.g., Fe2O3, Fe3O4 and α-/γ-FeOOH) and MnxOy (e.g., MnO2, Mn2O3 and their Ca, Na, and K mixed metal oxyhydrates todorokite (Ca,Na,K)2(Mn 3+/4+ )6O12·3-5H2O and birnessite (Na,Ca)Mn7O14⋅2-3H2O). Silica and iron oxide precursors mostly originate from the Earth's crust, while for manganese oxides the situation is a bit different: Although Mn(II) is also released through the weathering of igneous and metamorphic rocks, which through oxidation results in more than 30 known Mn(III), Mn(IV), or mixed Mn(III,IV) oxide/hydroxide minerals, manganese (and ferromanganese) oxides are more commonly found as nodules and crusts on the ocean floor ( Figure 2D). These nodules are typically brown-black spherical aggregates that consist of concentric layers of primarily MnO2 and iron oxide minerals (mostly
Weathering describes the breakdown of igneous, metamorphic and sedimentary rocks, through the action of water, temperature and biological activity. The mechanical, microbiological as well as chemical weathering lead the transformation of mineral rocks to so-called mineral soil. The minerals present in the soil are chemically altered in this process (see reactions I-III in Figure 2), releasing water-soluble ions into their surroundings. Through water circulation in and above ground, these species are transported to different loci and later are taken up by living organisms (for instance, through the roots of plants) as we will see later.
The three biogenic metal oxides are SiO 2 , Fe x O y (e.g., Fe 2 O 3 , Fe 3 O 4 and α-/γ-FeOOH) and Mn x O y (e.g., MnO 2 , Mn 2 O 3 and their Ca, Na, and K mixed metal oxyhydrates todorokite (Ca,Na,K) 2 (Mn 3+/4+ ) 6 O 12 ·3-5H 2 O and birnessite (Na,Ca)Mn 7 O 14 ·2-3H 2 O). Silica and iron oxide precursors mostly originate from the Earth's crust, while for manganese oxides the situation is a bit different: Although Mn(II) is also released through the weathering of igneous and metamorphic rocks, which through oxidation results in more than 30 known Mn(III), Mn(IV), or mixed Mn(III,IV) oxide/hydroxide minerals, manganese (and ferromanganese) oxides are more commonly found as nodules and crusts on the ocean floor ( Figure 2D). These nodules are typically brown-black spherical aggregates that consist of concentric layers of primarily MnO 2 and iron oxide minerals (mostly FeOOH) [21,22]. For ferromanganese nodules, microbial oxidation is an important weathering process. In the following section, we summarize the origins of precursors for all three biogenic metal oxides: silica (SiO 2 ), iron oxides (Fe x O y ) and manganese oxides (Mn x O y ).
Biomimetics 2020, 5, x FOR PEER REVIEW 5 of 39 FeOOH) [21,22]. For ferromanganese nodules, microbial oxidation is an important weathering process. In the following section, we summarize the origins of precursors for all three biogenic metal oxides: silica (SiO2), iron oxides (FexOy) and manganese oxides (MnxOy). license. Photograph of ferromanganese nodule is reproduced from [23] with permission from the Elsevier B.V.

Silicon Oxide
Silica is the most abundant MxOy in living nature. During silicate weathering in the presence of CO2, ortho-silicic acid Si(OH)4 is released from the crystalline structure of silicate minerals ( Figure 2A illustrates the weathering of anorthite to gibbsite as an example) [24]. In the environment, the Si(OH)4 dissolved in H2O is transported through the soil to rivers and the ocean. In water, at room temperature, Si(OH)4 and related species are stable for long periods of time at levels below ca. 100 ppm. However, once the concentration exceeds the solubility of the amorphous SiO2, around 100−200 ppm, it undergoes polycondensation reactions (see Figure 3A) [19]. Thus, silicic acid can precipitate as non-biogenic silica through self-condensation at >100-200 ppm. The precipitation of the silicic species generates silica (SiO2) which can be found either in amorphous (also known as opal, Figure  3B) or crystalline forms (e.g., quartz, cristobalite, tridymite, see Figure 1D). The variety and abundance of silicate minerals is a result of both the versatility and stability of silicon when bonded to oxygen, and the ease these SixOy structures incorporate other elements, forming a plethora of crystalline minerals [25]. Note that the geological weathering of the crystalline forms of silica requires millions of years.  [23] with permission from the Elsevier B.V.

Silicon Oxide
Silica is the most abundant M x O y in living nature. During silicate weathering in the presence of CO 2 , ortho-silicic acid Si(OH) 4 is released from the crystalline structure of silicate minerals ( Figure 2A illustrates the weathering of anorthite to gibbsite as an example) [24]. In the environment, the Si(OH) 4 dissolved in H 2 O is transported through the soil to rivers and the ocean. In water, at room temperature, Si(OH) 4 and related species are stable for long periods of time at levels below ca. 100 ppm. However, once the concentration exceeds the solubility of the amorphous SiO 2 , around 100−200 ppm, it undergoes polycondensation reactions (see Figure 3A) [19]. Thus, silicic acid can precipitate as non-biogenic silica through self-condensation at >100-200 ppm. The precipitation of the silicic species generates silica (SiO 2 ) which can be found either in amorphous (also known as opal, Figure 3B) or crystalline forms (e.g., quartz, cristobalite, tridymite, see Figure 1D). The variety and abundance of silicate minerals is a result of both the versatility and stability of silicon when bonded to oxygen, and the ease these Si x O y structures incorporate other elements, forming a plethora of crystalline minerals [25]. Note that the geological weathering of the crystalline forms of silica requires millions of years.
The precipitation of biogenic SiO 2 is fundamentally different from biominerals that are salts, such as CaCO 3 . The precipitation of salts is driven by solubility equilibria, while silica is an amorphous metal oxide formed by (inorganic) polymerization processes ( Figure 3A). Amorphous SiO 2 , in contrast to its crystalline analogs, exhibits no long-range order. It is built up from SiO 4 tetrahedra with Si-O-Si bonds, whose angles span over a broad range, and so do the Si-O bond distances. Amorphous SiO 2 is a covalent inorganic polymer. Often the general formula [SiO n/2 (OH) 4−n ] m (where n = 0-4) is used to account for not fully condensed species. Amorphous SiO 2 encompasses a broad variety of structural forms, from ordered opal aggregates to extended gel-like materials. Note that opal is built up of near-monodisperse spherical particles of hydrated silica (SiO 2 ·nH 2 O) which are arranged in an ordered hexagonal particle lattice (see Figure 3). Opals are 'mineraloids' since they do not fulfill all three criteria of minerals (crystallinity, inorganic nature, natural origin) that we have seen previously with respect to crystallinity. When a Si(OH) 4 solution is supersaturated, small particles are formed through condensation of monomers and small oligomers. Consequently, (hydrated) silica is precipitating until the supersaturation is relieved ( Figure 3A). Colloidal particles of silica are formed through the growth of the initial nuclei via further polycondensation. These, in turn, may be aggregated to form a silica gel (little interparticle order) or an opal (SiO 2 particle crystal), both of which bear surface Si-OH groups (see Figure 3B) [19].  The precipitation of biogenic SiO2 is fundamentally different from biominerals that are salts, such as CaCO3. The precipitation of salts is driven by solubility equilibria, while silica is an amorphous metal oxide formed by (inorganic) polymerization processes ( Figure 3A). Amorphous SiO2, in contrast to its crystalline analogs, exhibits no long-range order. It is built up from SiO4 tetrahedra with Si-O-Si bonds, whose angles span over a broad range, and so do the Si-O bond distances. Amorphous SiO2 is a covalent inorganic polymer. Often the general formula [SiOn/2(OH)4−n]m (where n = 0-4) is used to account for not fully condensed species. Amorphous SiO2 encompasses a broad variety of structural forms, from ordered opal aggregates to extended gel-like materials. Note that opal is built up of near-monodisperse spherical particles of hydrated silica (SiO2·nH2O) which are arranged in an ordered hexagonal particle lattice (see Figure 3). Opals are 'mineraloids' since they do not fulfill all three criteria of minerals (crystallinity, inorganic nature, natural origin) that we have seen previously with respect to crystallinity. When a Si(OH)4 solution is supersaturated, small particles are formed through condensation of monomers and small oligomers. Consequently, (hydrated) silica is precipitating until the supersaturation is relieved ( Figure 3A). Colloidal particles of silica are formed through the growth of the initial nuclei via further polycondensation. These, in turn, may be aggregated to form a silica gel (little interparticle order) or an opal (SiO2 particle crystal), both of which bear surface Si-OH groups (see Figure 3B) [19].
In biological organisms, silica exhibits no long-range order, irrespective of if it is found in simple organisms, animals or plants. These materials are all formed under ambient temperature and pressure and at circumneutral pH. Yet, many of the species are able to produce robust hierarchical structures through a process called biosilicification.
A comprehensive definition for biosilicification, i.e., the process of generating biogenic silica, is as: ''the movement of silicic acid from environments in which its concentration does not exceed its solubility (<2 mmol/L) to intracellular or systemic compartments in which it is accumulated for subsequent deposition as amorphous hydrated silica'' [26]. Biosilicification is largely studied for diatoms and sponges, which usually involves organic biomolecules such as proteins, peptides and small amines in stages crucial to biosilica formation, such as Si uptake, transport and deposition. Combining approaches from molecular biology, genetics and cell biology, researchers have unveiled mechanistic aspects of biosilica formation in these systems. Examples include the identification of silicon transporters which are postulated to actively uptake silicic acid from the environment into the silicifying organisms [27], propylamines found in diatoms and sponges that have been shown to rapidly precipitate silica in in vitro in model reactions [28], and silicatein proteins from a range of In biological organisms, silica exhibits no long-range order, irrespective of if it is found in simple organisms, animals or plants. These materials are all formed under ambient temperature and pressure and at circumneutral pH. Yet, many of the species are able to produce robust hierarchical structures through a process called biosilicification.
A comprehensive definition for biosilicification, i.e., the process of generating biogenic silica, is as: "the movement of silicic acid from environments in which its concentration does not exceed its solubility (<2 mmol/L) to intracellular or systemic compartments in which it is accumulated for subsequent deposition as amorphous hydrated silica" [26]. Biosilicification is largely studied for diatoms and sponges, which usually involves organic biomolecules such as proteins, peptides and small amines in stages crucial to biosilica formation, such as Si uptake, transport and deposition. Combining approaches from molecular biology, genetics and cell biology, researchers have unveiled mechanistic aspects of biosilica formation in these systems. Examples include the identification of silicon transporters which are postulated to actively uptake silicic acid from the environment into the silicifying organisms [27], propylamines found in diatoms and sponges that have been shown to rapidly precipitate silica in in vitro in model reactions [28], and silicatein proteins from a range of silica sponges [29][30][31]. We are detailing the SiO 2 formation on living organisms in Section 2.1, for the different SiO 2 -mineralizing species.

Iron Oxides
Iron is released to the environment by the weathering of Fe 2+ -containing silicates (e.g., biotite, pyroxene, amphibole, olivine). Figure 2A illustrates the chemical weathering of the iron silicate olivine. Weathering of iron minerals is usually aided by microorganisms. Dissolved Fe 2+ (so-called 'ferrous' iron) oxidizes spontaneously to Fe 3+ ('ferric' iron), which in turn instantaneously reacts with water to form Biomimetics 2020, 5, 29 7 of 36 amorphous ferrihydrite (which is an iron oxyhydroxide, see Reaction 1) [32]. As we will see later, living organisms can transform these Fe 3+ oxyhydroxides into crystalline structures. (see Reaction 1. Reaction equation of the oxidation of ferrous ions to ferric oxide): Among the crystalline forms of iron oxides, lepidocrocite (γ-FeOOH), goethite (α-FeOOH) and magnetite (Fe 3 O 4 ) have been found in living species together with some amorphous oxy-hydroxides, Figure 4 (note that according to the Strunz classification, hydroxides (and oxyhydroxides) are considered oxide minerals [32]. Moreover, in accordance with Strunz Mineralogical Tables, we herein adopted the form FeOOH to represent oxyhydroxides instead of the sometimes also used FeO(OH)). The most studied iron biomineral is magnetite ( Figure 4D), which has a cubic, inverse spinel structure and is ferrimagnetic, i.e., it presents permanent magnetism, at ambient temperature [33]. Their incorporation into living organisms will be discussed in Section 2.3.

Iron Oxides
Iron is released to the environment by the weathering of Fe 2+ -containing silicates (e.g., biotite, pyroxene, amphibole, olivine). Figure 2A illustrates the chemical weathering of the iron silicate olivine. Weathering of iron minerals is usually aided by microorganisms. Dissolved Fe 2+ (so-called 'ferrous' iron) oxidizes spontaneously to Fe 3+ ('ferric' iron), which in turn instantaneously reacts with water to form amorphous ferrihydrite (which is an iron oxyhydroxide, see Reaction 1) [32]. As we will see later, living organisms can transform these Fe 3+ oxyhydroxides into crystalline structures. 4Fe 2+ + O2 + 6H2O → 4FeOOH + 8H + Reaction 1. Reaction equation of the oxidation of ferrous ions to ferric oxide.
Among the crystalline forms of iron oxides, lepidocrocite (γ-FeOOH), goethite (α-FeOOH) and magnetite (Fe3O4) have been found in living species together with some amorphous oxy-hydroxides, Figure 4 (note that according to the Strunz classification, hydroxides (and oxyhydroxides) are considered oxide minerals [32]. Moreover, in accordance with Strunz Mineralogical Tables, we herein adopted the form FeOOH to represent oxyhydroxides instead of the sometimes also used FeO(OH)). The most studied iron biomineral is magnetite ( Figure 4D), which has a cubic, inverse spinel structure and is ferrimagnetic, i.e., it presents permanent magnetism, at ambient temperature [33]. Their incorporation into living organisms will be discussed in Section 2.3.

Manganese Oxides
Mn is released by weathering of Mn 2+ -containing silicates (e.g., biotite, pyroxene, amphibole) and leaching of ferromanganese nodules. As for the Fe oxides, the weathering of Mn minerals is heavily supported by microbial activity. Bacteria catalyze the oxidation of Mn 2+ by indirect and direct processes. Indirect oxidation of Mn 2+ occurs when organisms modify the pH and/or redox conditions of the local aqueous environment, or by the release of metabolic products that chemically oxidize Mn 2+ . In the direct process, bacteria oxidize Mn 2+ through the production of polysaccharides or proteins [21]. The elucidation of the biochemical process involved in Mn 2+ oxidation has only been recently achieved and will be detailed later on. Biogenic manganese oxides are mainly found in bacteria and fungi, and occur in many cases as crystalline layered birnessite ((Na,Ca)Mn7O14·2-3H2O) or tunnel-type todorokite ((Ca,Na,K)2(Mn 3+/4+ )6O12·3-5H2O); see Figure 5, further discussed in Section 2.4.

Manganese Oxides
Mn is released by weathering of Mn 2+ -containing silicates (e.g., biotite, pyroxene, amphibole) and leaching of ferromanganese nodules. As for the Fe oxides, the weathering of Mn minerals is heavily supported by microbial activity. Bacteria catalyze the oxidation of Mn 2+ by indirect and direct processes. Indirect oxidation of Mn 2+ occurs when organisms modify the pH and/or redox conditions of the local aqueous environment, or by the release of metabolic products that chemically oxidize Mn 2+ . In the direct process, bacteria oxidize Mn 2+ through the production of polysaccharides or proteins [21]. The elucidation of the biochemical process involved in Mn 2+ oxidation has only been recently achieved and will be detailed later on. Biogenic manganese oxides are mainly found in bacteria and fungi, and occur in many cases as crystalline layered birnessite ((Na,Ca)Mn 7 O 14 ·2-3H 2 O) or tunnel-type todorokite ((Ca,Na,K) 2 (Mn 3+/4+ ) 6 O 12 ·3-5H 2 O); see Figure 5, further discussed in Section 2.4.

The Biogenesis of Metal Oxides
Silica is the second most abundant MxOy biomineral after carbonates. Related ferric oxide minerals rank in the fourth most extensively formed biogenic MxOy. Manganese oxides are much less abundant than Si and Fe oxides, and are mainly found in bacteria and fungi. Figure 6 lists examples of biogenic MxOy. The table is organized according to their distribution in the phyla of the five kingdoms [5]. For specific taxa in certain phyla, please consult [8]. From Figure  6, it becomes clear that silica and iron oxides are the most representative MxOy in living nature and are widely distributed among the kingdoms. In terms of structures formed, opal (amorphous SiO2) is

The Biogenesis of Metal Oxides
Silica is the second most abundant M x O y biomineral after carbonates. Related ferric oxide minerals rank in the fourth most extensively formed biogenic M x O y . Manganese oxides are much less abundant than Si and Fe oxides, and are mainly found in bacteria and fungi. Figure 6 lists examples of biogenic M x O y . The table is organized according to their distribution in the phyla of the five kingdoms [5]. For specific taxa in certain phyla, please consult [8]. From Figure 6, it becomes clear that silica and iron oxides are the most representative M x O y in living nature and are widely distributed among the kingdoms. In terms of structures formed, opal (amorphous SiO 2 ) is clearly the most abundant, followed by iron oxides, particularly magnetite.

Silicon Dioxide
Biogenic silicas are the product of biological processes that lead to the formation of composite materials of diverse composition, hierarchical structures, and functions. SiO2 is found in various organisms ranging from bacteria to plants. In the following, we will focus on examples of silica present in bacteria and fungi, plantae and animalia kingdoms.

Silicon Dioxide
Biogenic silicas are the product of biological processes that lead to the formation of composite materials of diverse composition, hierarchical structures, and functions. SiO 2 is found in various organisms ranging from bacteria to plants. In the following, we will focus on examples of silica present in bacteria and fungi, plantae and animalia kingdoms.
Microbes, irrespective of where they live, commonly act as templates for the nucleation and precipitation of amorphous silica (opal-A) and other minerals through the reactive sites that exist on their surfaces [79]. Microbial mineralization is commonly associated with hydrothermal vents on land, lake floors, and the seafloor. Here, the waters originating from deep hot reservoirs containing besides other metallic species, dissolved silicic acids. When these fluids are discharged at the surface, rapid cooling to ambient temperatures, evaporation, and changes in the pH of the solutions cause the sudden surpassing of the solubility of amorphous SiO 2 . This prompts monomeric ortho-silicic acid, Si(OH) 4 , to polymerize, initially to oligomers and then to polymeric species, which further precipitate as amorphous hydrated silica. These freshly precipitated (hydrated) SiO 2 species are commonly referred to as 'sinters' [80].
Most siliceous sinters contain silicified microorganisms. For example, Jones et al. have reported silicified microbe mats ( Figure 7B) found in chimneys of submarine volcanoes ( Figure 7A), and analyzed these with respect to their morphology and biogenicity [79]. Although DNA analyses of the samples were inconclusive, the authors showed that the mineralized microbes in the samples are formed of at least three different types of opal-A morphologies ( Figure 7C-E), i.e., filamentous microbes, rod-shaped microbes and spherical microbes. Complementarily, the work of Konhauser et al. on silicified bacteria from a geyser outflow channel shows microbial cells encrusted in spheroidal grains of silica extracellularly on the sheaths or walls of living cells ( Figure 7F) [80]. Microbes, irrespective of where they live, commonly act as templates for the nucleation and precipitation of amorphous silica (opal-A) and other minerals through the reactive sites that exist on their surfaces [79]. Microbial mineralization is commonly associated with hydrothermal vents on land, lake floors, and the seafloor. Here, the waters originating from deep hot reservoirs containing besides other metallic species, dissolved silicic acids. When these fluids are discharged at the surface, rapid cooling to ambient temperatures, evaporation, and changes in the pH of the solutions cause the sudden surpassing of the solubility of amorphous SiO2. This prompts monomeric ortho-silicic acid, Si(OH)4, to polymerize, initially to oligomers and then to polymeric species, which further precipitate as amorphous hydrated silica. These freshly precipitated (hydrated) SiO2 species are commonly referred to as 'sinters' [80].
Most siliceous sinters contain silicified microorganisms. For example, Jones et al. have reported silicified microbe mats ( Figure 7B) found in chimneys of submarine volcanoes ( Figure 7A), and analyzed these with respect to their morphology and biogenicity [79]. Although DNA analyses of the samples were inconclusive, the authors showed that the mineralized microbes in the samples are formed of at least three different types of opal-A morphologies ( Figure   (E) Silicified rod-shaped microbes coated with opal-A and scattered opal-A spheres. (F) TEM cut of silicified bacteria from a geyser outflow channel, showing a filamentous cyanobacterium with silica spheroids on outer sheath (arrows). Images A-E are adapted from [79] with permission from John Wiley and Sons. Image F is reproduced from [80] with permission from Springer Nature BV.
Moreover, a number of silicates associated with Fe and Al oxides of clay-type have been observed on the surface of bacterial envelopes in different environments. The metal content of the clays is usually reflecting the metals present in the surrounding water. In river sediments [81], hot springs [82], and mine tailings [83], silicate minerals of usually a clay-like composition and structure are found in association with bacteria [84]. The silicate deposits in these microbes are found as thin (~100 nm) crusts on and around the bacteria cells ( Figure 8). It is likely that the bacteria play an Moreover, a number of silicates associated with Fe and Al oxides of clay-type have been observed on the surface of bacterial envelopes in different environments. The metal content of the clays is usually reflecting the metals present in the surrounding water. In river sediments [81], hot springs [82], and mine tailings [83], silicate minerals of usually a clay-like composition and structure are found in association with bacteria [84]. The silicate deposits in these microbes are found as thin (~100 nm) crusts on and around the bacteria cells ( Figure 8). It is likely that the bacteria play an important role in their formation, rather than simply binding pre-formed minerals detritus, since (i) the composition of silicates found on the cells differs markedly from those silicates not associated with bacterial cells, and (ii) the silicate precipitates found on the cell are more crystalline and larger in structure. Interestingly, even in environments with low Si(OH) 4 concentrations, such as freshwater lakes and rivers, clay-like precipitates are found on bacterial cells.
the composition of silicates found on the cells differs markedly from those silicates not associated with bacterial cells, and (ii) the silicate precipitates found on the cell are more crystalline and larger in structure. Interestingly, even in environments with low Si(OH)4 concentrations, such as freshwater lakes and rivers, clay-like precipitates are found on bacterial cells.
A possible process for the formation of silica in this context involves the direct interaction of soluble anionic silicates with the positively charged groups on the peptidoglycan (a polymer of sugars and amino acids that shapes the cell wall) of the bacterial envelopes, such as the amine side groups on the peptide chain. Hydrogen bonding between silanol groups and the polysaccharide hydroxy groups of the cell wall may also be involved. If the superficial bacterial layers are predominantly negatively charged, external cations (Al, Fe) can interact with the cell wall and also provide nucleation sites for the mineralization [85,86]. A combination of these processes seems to be involved in the formation of silica at the surface of the Gram-positive bacterium Bacillus subtilis [85] and Gram-negative Thiobacillusin [83] mine tailings. This coating is often associated with extreme environments, which suggests that it may also serve as a protecting shell for the bacteria. Reproduced from [84] with permission from Elsevier.

Sponges (Kingdom Animalia, Phylum Porifera)
Sponges, members of the phylum porifera, are multicellular organisms that have porous and opened-channel silica bodies of a plethora of morphologies, that allows circulation of water through their bodies. Like diatoms, sponges produce a variety of skeletons and they are classified into three classes: Hexactinellida, Desmospongiae and Calcarea. Although all three utilize biomineralization in forming their skeletons, only Hexactinellida and Desmospongiae do so using silicon to build robust structures of silica while Calcerea utilize calcium carbonate [8]. The chemical composition of demosponge and hexactinellid spicules varies slightly depending on the species and the water composition in the habitat, but it is mostly silica (SiO2), and water, with some trace elements [87]. Sponges take up silicon in the form of soluble silicic acid to form spicules. Si uptake by sponges has been measured in laboratory experiments and may vary according to the Si concentration in the water, the temperature, and other environmental factors that affect sponge physiology and metabolism [29].
For providing a perspective for the MxOy biominerals reviewed in this work, we are in the following summarizing the biomolecules involved in sponge silica formation. As we think that biosilicification process can serve as biomimetic inspiration for the synthesis of SiO2 (see perspective Section 3), we have decided to in the following summarize the involved process from a A possible process for the formation of silica in this context involves the direct interaction of soluble anionic silicates with the positively charged groups on the peptidoglycan (a polymer of sugars and amino acids that shapes the cell wall) of the bacterial envelopes, such as the amine side groups on the peptide chain. Hydrogen bonding between silanol groups and the polysaccharide hydroxy groups of the cell wall may also be involved. If the superficial bacterial layers are predominantly negatively charged, external cations (Al, Fe) can interact with the cell wall and also provide nucleation sites for the mineralization [85,86]. A combination of these processes seems to be involved in the formation of silica at the surface of the Gram-positive bacterium Bacillus subtilis [85] and Gram-negative Thiobacillusin [83] mine tailings. This coating is often associated with extreme environments, which suggests that it may also serve as a protecting shell for the bacteria.

Sponges (Kingdom Animalia, Phylum Porifera)
Sponges, members of the phylum porifera, are multicellular organisms that have porous and opened-channel silica bodies of a plethora of morphologies, that allows circulation of water through their bodies. Like diatoms, sponges produce a variety of skeletons and they are classified into three classes: Hexactinellida, Desmospongiae and Calcarea. Although all three utilize biomineralization in forming their skeletons, only Hexactinellida and Desmospongiae do so using silicon to build robust structures of silica while Calcerea utilize calcium carbonate [8]. The chemical composition of demosponge and hexactinellid spicules varies slightly depending on the species and the water composition in the habitat, but it is mostly silica (SiO 2 ), and water, with some trace elements [87]. Sponges take up silicon in the form of soluble silicic acid to form spicules. Si uptake by sponges has been measured in laboratory experiments and may vary according to the Si concentration in the water, the temperature, and other environmental factors that affect sponge physiology and metabolism [29].
For providing a perspective for the M x O y biominerals reviewed in this work, we are in the following summarizing the biomolecules involved in sponge silica formation. As we think that biosilicification process can serve as biomimetic inspiration for the synthesis of SiO 2 (see perspective Section 3), we have decided to in the following summarize the involved process from a chemical/synthetic point of view. Note that the biosilicification processes of diatoms and sponges have been reviewed in great detail in [3,10,15,29,88,89].
A major breakthrough in the understanding of biosilicification of the silica-spicule, a sharp-pointed structure occurring in the skeleton of a sponge, was prompted through the discovery of a key enzyme. Morse et al. discovered that the organic filament in the central canal of the spicules is composed of a cathepsin L-related enzyme, which are termed silicatein ( Figure 9) [90,91].
Biomimetics 2020, 5, x FOR PEER REVIEW 12 of 39 chemical/synthetic point of view. Note that the biosilicification processes of diatoms and sponges have been reviewed in great detail in [3,10,15,29,88,89]. A major breakthrough in the understanding of biosilicification of the silica-spicule, a sharppointed structure occurring in the skeleton of a sponge, was prompted through the discovery of a key enzyme. Morse et al. discovered that the organic filament in the central canal of the spicules is composed of a cathepsin L-related enzyme, which are termed silicatein ( Figure 9) [90,91]. The mechanism of the silicatein catalyzed polymerization of Si(OH)4 to SiO2 relies on the assumption that the presence of both the serine and histidine residue in the catalytic centre of silicatein are essential for the interaction with the substrate orthosilicic acid and the subsequent polymerization. One of the proposed catalytic mechanisms is described in Figure 10 [30].
The following process proceeds in the catalytic pocket of silicatein ( Figure 10): (i) in the first step, a nucleophilic attack (SN2-type) of the (electronegative) O of the serine residue's OH group to the (electropositive) Si atom of a Si(OH)4 molecule (step 1). This mechanism is facilitated by the H-bond between the Ser and the His residues, which increases the nucleophilicity of the serine's OH group. Then, the H-transfer from the Ser-His H-bond to one of the OH ligands of Si(OH)4 occurs, forming a pentavalent intermediate and the serine residue is positioned in the catalytic centre of silicatein. (ii) After release of water (step 2), this serine-bound silicic acid molecule undergoes a nucleophilic attack at the silicon atom of a second Si(OH)4 molecule and generates a disilicic acid molecule (step 3) that is bound to silicatein. (iii) Then, the rotation of the Si-O-Ser bond is required to allow an interaction of a second OH ligand of the enzyme-bound silicic acid unit with the nitrogen imidazole of the catalytic centre His residue (step 4), facilitating further growth of the disilicic acid by nucleophilic attack to a third Si(OH)4 molecule (step 5). (iv) Several repetitions of the reaction cycle (SN2-type attack, H-transfer, loss of water, rotation) result in higher membered silicic acid oligomers. (v) The covalent linkage between the enzyme and the silicic acid oligomer is hydrolyzed by water (step 6), thus freeing the enzyme pocket. The mechanism of the silicatein catalyzed polymerization of Si(OH) 4 to SiO 2 relies on the assumption that the presence of both the serine and histidine residue in the catalytic centre of silicatein are essential for the interaction with the substrate orthosilicic acid and the subsequent polymerization. One of the proposed catalytic mechanisms is described in Figure 10 [30].
Biomimetics 2020, 5, x FOR PEER REVIEW 13 of 39 Figure 10. The proposed mechanism of silicatein-catalyzed polymerization of orthosilicic acid. Note that the example shown as product is a trisiloxane (SiO)3(OH)6. Adapted from [30] with permission from Springer Nature.
Spicules are of particular interest. These structures consist of glassy rods with diameters ranging from a few microns to several mm, and enormous lengths reaching up to 3 m [92]. They exhibit high fracture toughness and low elastic moduli, which leads to outstanding flexibilities for which there is no equivalent amongst synthetic silica-based materials. Spicules can present diverse morphologies as illustrated in Figure 11. They are used for structuring the skeleton, defense, food entrapment, and anchoring of the sponge on the seafloor. As it has been shown for diatoms, spicule synthesis and morphologies are both genetically encoded and influenced by environmental factors such as wave Figure 10. The proposed mechanism of silicatein-catalyzed polymerization of orthosilicic acid. Note that the example shown as product is a trisiloxane (SiO) 3 (OH) 6 . Adapted from [30] with permission from Springer Nature.
The following process proceeds in the catalytic pocket of silicatein ( Figure 10): (i) in the first step, a nucleophilic attack (S N 2-type) of the (electronegative) O of the serine residue's OH group to the (electropositive) Si atom of a Si(OH) 4 molecule (step 1). This mechanism is facilitated by the H-bond between the Ser and the His residues, which increases the nucleophilicity of the serine's OH group. Then, the H-transfer from the Ser-His H-bond to one of the OH ligands of Si(OH) 4 occurs, forming a pentavalent intermediate and the serine residue is positioned in the catalytic centre of silicatein. (ii) After release of water (step 2), this serine-bound silicic acid molecule undergoes a nucleophilic attack at the silicon atom of a second Si(OH) 4 molecule and generates a disilicic acid molecule (step 3) that is bound to silicatein. (iii) Then, the rotation of the Si-O-Ser bond is required to allow an interaction of a second OH ligand of the enzyme-bound silicic acid unit with the nitrogen imidazole of the catalytic centre His residue (step 4), facilitating further growth of the disilicic acid by nucleophilic attack to a third Si(OH) 4 molecule (step 5). (iv) Several repetitions of the reaction cycle (S N 2-type attack, H-transfer, loss of water, rotation) result in higher membered silicic acid oligomers.
(v) The covalent linkage between the enzyme and the silicic acid oligomer is hydrolyzed by water (step 6), thus freeing the enzyme pocket.
Spicules are of particular interest. These structures consist of glassy rods with diameters ranging from a few microns to several mm, and enormous lengths reaching up to 3 m [92]. They exhibit high fracture toughness and low elastic moduli, which leads to outstanding flexibilities for which there is no equivalent amongst synthetic silica-based materials. Spicules can present diverse morphologies as illustrated in Figure 11. They are used for structuring the skeleton, defense, food entrapment, and anchoring of the sponge on the seafloor. As it has been shown for diatoms, spicule synthesis and morphologies are both genetically encoded and influenced by environmental factors such as wave forces and local silicon concentrations [87]. Spicules are made of concentric layers of hydrated amorphous silica surrounding an axial proteic filament ( Figure 12). This filament does not only template silica deposition but also catalyzes the polymerization of silicic acid species [87,93]. The morphological, physical, and chemical characteristics of spicules were extensively analyzed by Müller and coworkers, using optical and electron microscopy and high resolution nuclear magnetic resonance [29,30,89,94,95]. It could be demonstrated that spicule formation starts within specialized cells, the sclerocytes, around the axial filament. After the silica layer around the axial filament reaches a diameter of approximately 3-5 μm, this layer becomes surrounded by organic silicatein, which synthesizes the second siliceous layer, and this process is repeated many times until many concentric layers are formed. If the formation of siliceous spicules is inhibited, the sponge body collapses. Aside silicateins, other proteins such as galectin and silicase are believed to be necessary for the synthesis of spicules [96]. Galectin binds silicatein and forms an organized net-like matrix on the surface of the spicules, while silicase is able to depolymerize amorphous silica and thereby allows for corrections in the skeleton formation [97]. Spicules are made of concentric layers of hydrated amorphous silica surrounding an axial proteic filament ( Figure 12). This filament does not only template silica deposition but also catalyzes the polymerization of silicic acid species [87,93]. The morphological, physical, and chemical characteristics of spicules were extensively analyzed by Müller and coworkers, using optical and electron microscopy and high resolution nuclear magnetic resonance [29,30,89,94,95]. It could be demonstrated that spicule formation starts within specialized cells, the sclerocytes, around the axial filament. After the silica layer around the axial filament reaches a diameter of approximately 3-5 µm, this layer becomes surrounded by organic silicatein, which synthesizes the second siliceous layer, and this process is repeated many times until many concentric layers are formed. If the formation of siliceous spicules is inhibited, the sponge body collapses. Aside silicateins, other proteins such as galectin and silicase are believed to be necessary for the synthesis of spicules [96]. Galectin binds silicatein and forms an organized net-like matrix on the surface of the spicules, while silicase is able to depolymerize amorphous silica and thereby allows for corrections in the skeleton formation [97]. The spicule skeleton of sponges is of a highly complex architecture with the spicules being glued together by a collagenous 'cement' [98]. In rare cases, chitin is used instead of collagen as a binder [99]. The most beautiful examples of such complex architectures are glass-sponges (hexactinellida), e.g., in Euplectella aspergillum ( Figure 13A). From the micrograph displayed in Figure 13B, taken inside the sponge skeleton, it can be seen that the spicule-network renders a well-defined shape. Their spicules grow to larger sizes and fuse to form a continuous super-scaffold ( Figure 13C). These complex spicule frameworks are in fact used as a light transmission system, as described in the following section [100]. The spicule skeleton of sponges is of a highly complex architecture with the spicules being glued together by a collagenous 'cement' [98]. In rare cases, chitin is used instead of collagen as a binder [99]. The most beautiful examples of such complex architectures are glass-sponges (hexactinellida), e.g., in Euplectella aspergillum ( Figure 13A). From the micrograph displayed in Figure 13B, taken inside the sponge skeleton, it can be seen that the spicule-network renders a well-defined shape. Their spicules grow to larger sizes and fuse to form a continuous super-scaffold ( Figure 13C). These complex spicule frameworks are in fact used as a light transmission system, as described in the following section [100]. The spicule skeleton of sponges is of a highly complex architecture with the spicules being glued together by a collagenous 'cement' [98]. In rare cases, chitin is used instead of collagen as a binder [99]. The most beautiful examples of such complex architectures are glass-sponges (hexactinellida), e.g., in Euplectella aspergillum ( Figure 13A). From the micrograph displayed in Figure 13B, taken inside the sponge skeleton, it can be seen that the spicule-network renders a well-defined shape. Their spicules grow to larger sizes and fuse to form a continuous super-scaffold ( Figure 13C). These complex spicule frameworks are in fact used as a light transmission system, as described in the following section [100].

Light-Harvesting in Sponges
The function of sponge spicules as optical waveguides was first described by Cattaneo-Vietti et al. in 1996 [101]. They showed that siliceous spicules from Rossella racovitzae, a hexactinellid species, act as light-collecting optical fibers. A decade later, Müller and coworkers showed that only light between 615 and 1310 nm (visible and near-infrared regions, respectively) can pass through the spicules of hexactinellid Hyalonema sieboldii [102], and spicules of Monorhapsis sp [103]. Although there is a substantial body of evidence that silica spicules present interesting optical properties, only few species exhibiting light harvesting and transmitting functions have been reported. It was found that sponge spicules can show long-lived fluorescence with a maximum at 770 nm and strong optical nonlinear behavior when pumped with femtosecond laser pulses [104]. Recently, a study concluded that the spicules of Sericolophus hawaiicus sponges might act as a natural supercontinuum generator (supercontinuum generation is a combination of nonlinear optical effects that spectrally broaden an initially nearly monochromatic laser beam, and it is used to provide intense sources of white light [105]), involving wavelengths between 650 and 900 nm [106]. This optical property was assumed to be possible through the spicules' composite nature, i.e., have a combination of silica and an organic matrix. In fact, the speculations about a possible light reception system were confirmed by Müller and coworkers [100]. For the first time, Müller and coworkers reported that the demosponge Suberites domuncula exhibits a synergistic interaction of their siliceous spicule system with a biosensor system consisting of a light releasing luciferase. The light-generating luciferase protein has been identified, and it was shown that the luciferase together with the inorganic spicule acts as waveguides for the transmission of light and electrical and chemical signals, similar to a 'neuron-like' network system [103,107].
Further investigations revealed that not only light generated within the interior of the sponges by luciferases might be present [108]. Other substances have been shown to be involved in light harvesting. The S. domuncula sponge ( Figure 14A) displays spicules of 150-320 µm on their surface, with a globular swelling at one end and a pointy tip at the other end ( Figure 14B). The authors assume that the globular siliceous ends act as convex lenses that focus the light. The authors identified the red colored compounds in the sponge tissues as carotenoids with spectral maxima at 400 and 430 nm. The reddish-yellow color of the sponge comes from the degradation products of β-carotene to b-cyclocitral and crocetin ( Figure 14C). Sponges of type S. domuncula are assumed to collect the light within the spherical knobs of their spicules, and guide it through the spicules into the interior of the organism. The carotenoid pigments seem to play a dual role: (i) they are involved in certain metabolic activities, and (ii) act as a sensitizers and dopants for the silica-spicule light waveguide [100].

Light-Harvesting in Sponges
The function of sponge spicules as optical waveguides was first described by Cattaneo-Vietti et al. in 1996 [101]. They showed that siliceous spicules from Rossella racovitzae, a hexactinellid species, act as light-collecting optical fibers. A decade later, Müller and coworkers showed that only light between 615 and 1310 nm (visible and near-infrared regions, respectively) can pass through the spicules of hexactinellid Hyalonema sieboldii [102], and spicules of Monorhapsis sp [103]. Although there is a substantial body of evidence that silica spicules present interesting optical properties, only few species exhibiting light harvesting and transmitting functions have been reported. It was found that sponge spicules can show long-lived fluorescence with a maximum at 770 nm and strong optical nonlinear behavior when pumped with femtosecond laser pulses [104]. Recently, a study concluded that the spicules of Sericolophus hawaiicus sponges might act as a natural supercontinuum generator (supercontinuum generation is a combination of nonlinear optical effects that spectrally broaden an initially nearly monochromatic laser beam, and it is used to provide intense sources of white light [105]), involving wavelengths between 650 and 900 nm [106]. This optical property was assumed to be possible through the spicules' composite nature, i.e., have a combination of silica and an organic matrix. In fact, the speculations about a possible light reception system were confirmed by Müller and coworkers [100]. For the first time, Müller and coworkers reported that the demosponge Suberites domuncula exhibits a synergistic interaction of their siliceous spicule system with a biosensor system consisting of a light releasing luciferase. The light-generating luciferase protein has been identified, and it was shown that the luciferase together with the inorganic spicule acts as waveguides for the transmission of light and electrical and chemical signals, similar to a 'neuron-like' network system [103,107].
Further investigations revealed that not only light generated within the interior of the sponges by luciferases might be present [108]. Other substances have been shown to be involved in light harvesting. The S. domuncula sponge ( Figure 14A) displays spicules of 150-320 μm on their surface, with a globular swelling at one end and a pointy tip at the other end ( Figure 14B). The authors assume that the globular siliceous ends act as convex lenses that focus the light. The authors identified the red colored compounds in the sponge tissues as carotenoids with spectral maxima at 400 and 430 nm. The reddish-yellow color of the sponge comes from the degradation products of β-carotene to bcyclocitral and crocetin ( Figure 14C). Sponges of type S. domuncula are assumed to collect the light within the spherical knobs of their spicules, and guide it through the spicules into the interior of the organism. The carotenoid pigments seem to play a dual role: (i) they are involved in certain metabolic activities, and (ii) act as a sensitizers and dopants for the silica-spicule light waveguide [100].

Plants (Kingdom Plantae)
Terrestrial plants such as grasses, bamboo, and certain tropical trees, absorb large quantities of silicon from the soil and deposit it as hydrated amorphous silica in different tissues, from the roots to the stems and leaves ( Figure 15A) [109][110][111]. In grasses, silica is deposited in all the organs, and the highest level of silicification is usually found in the inflorescence epidermis ( Figure 15B-C), leaves ( Figure 15D-E) and in the root (Figure 15F-G) [112]. Note the following definition: Inflorescence: the shoot of seed plants where flowers are formed, i.e., the reproductive portion of a plant. Glume: each of two bracts (a leaf-like structure) surrounding the grass flower (known as spikelet). Lemma: bracts at the base of each individual small flower (floret) clustered within an inflorescence. See detail in Figure 15A.

Plants (Kingdom Plantae)
Terrestrial plants such as grasses, bamboo, and certain tropical trees, absorb large quantities of silicon from the soil and deposit it as hydrated amorphous silica in different tissues, from the roots to the stems and leaves ( Figure 15A) [109][110][111]. In grasses, silica is deposited in all the organs, and the highest level of silicification is usually found in the inflorescence epidermis ( Figure 15B-C), leaves ( Figure 15D-E) and in the root ( Figure 15F-G) [112]. Note the following definition: Inflorescence: the shoot of seed plants where flowers are formed, i.e., the reproductive portion of a plant. Glume: each of two bracts (a leaf-like structure) surrounding the grass flower (known as spikelet). Lemma: bracts at the base of each individual small flower (floret) clustered within an inflorescence. See detail in Figure 15A.  SiO 2 structures are found in the inflorescence bracts, and serve as a hard-protecting shell to the development of the seed. Specifically, SiO 2 is concentrated on the prickles and papillae cells (indicated by red arrows in Figure 15B-C) on the glume and lemma 8 structures. Cells found in the leaf accumulate silica in their walls as well. Since leaves are remarkably involved in plant transpiration, the evaporation of water promotes the condensation of silica in these structures. Figure 15D-E illustrates the cross-section micrographs of a leaf, showing silica bodies in the leaf's epidermis and tip, respectively (indicated by red arrow). The deposition of silica also extends to the root's region, the first organ exposed to Si(OH) 4 present in the soil. In Figure 15F-G, one can observe the presence of larger aggregates of silica along the cell walls of the root's endodermis (indicated by red arrows).
Once silicic species are taken up by the roots, they are transported to and deposited inside the cells, in the cell walls (as exemplified before) and in extracellular spaces of stems and leaves as hydrous amorphous silica particles, so-called phytoliths ( Figure 16). Unlike for diatoms and sponges where silica deposition is much better understood, there have been contrasting hypotheses to explain silica deposition in plants, in particular to understand the formation of phytoliths [113]. One of the most accepted hypotheses is the passive silicification that relies on the silica deposition by organ transpiration, which implies that this is a spontaneous process resulting from auto-condensation of Si(OH) 4 as water evaporates. Another hypothesis involves an enzymatic catalysis, or even a combination of both approaches [112].
In the passive silicification in plants, soluble silica in the soil is usually present as silicic acid Si(OH) 4 and it is taken up by the roots and transported through the xylem (the tissue responsible for transporting water and dissolved compounds from roots to stems and leaves). Silicic acid species (e.g., Si(OH) 4 , (OH) 3 Si-O-Si-(OH) 3 , [SiO n/2 (OH) 4-n ] m ) are transported through the plant to a deposition site (the cell wall, the cell lumen and in intercellular and extracellular spaces) where the silica concentration is raised to the extent that it precipitates out to form a solid hydrated silica body ( Figure 16A) [109,114]. The silica bodies, the phytoliths, exhibit interesting morphologies as illustrated in Figure 16B. Although amorphous silica has only short-range order, cellulose and other carbohydrates are ordered structures, and therefore impart a certain shape on the silica that is deposited [3].
SiO2 structures are found in the inflorescence bracts, and serve as a hard-protecting shell to the development of the seed. Specifically, SiO2 is concentrated on the prickles and papillae cells (indicated by red arrows in Figure 15B-C) on the glume and lemma 8 structures. Cells found in the leaf accumulate silica in their walls as well. Since leaves are remarkably involved in plant transpiration, the evaporation of water promotes the condensation of silica in these structures. Figure  15D-E illustrates the cross-section micrographs of a leaf, showing silica bodies in the leaf's epidermis and tip, respectively (indicated by red arrow). The deposition of silica also extends to the root's region, the first organ exposed to Si(OH)4 present in the soil. In Figure 15F-G, one can observe the presence of larger aggregates of silica along the cell walls of the root's endodermis (indicated by red arrows).
Once silicic species are taken up by the roots, they are transported to and deposited inside the cells, in the cell walls (as exemplified before) and in extracellular spaces of stems and leaves as hydrous amorphous silica particles, so-called phytoliths ( Figure 16). Unlike for diatoms and sponges where silica deposition is much better understood, there have been contrasting hypotheses to explain silica deposition in plants, in particular to understand the formation of phytoliths [113]. One of the most accepted hypotheses is the passive silicification that relies on the silica deposition by organ transpiration, which implies that this is a spontaneous process resulting from auto-condensation of Si(OH)4 as water evaporates. Another hypothesis involves an enzymatic catalysis, or even a combination of both approaches [112].
In the passive silicification in plants, soluble silica in the soil is usually present as silicic acid Si(OH)4 and it is taken up by the roots and transported through the xylem (the tissue responsible for transporting water and dissolved compounds from roots to stems and leaves). Silicic acid species (e.g., Si(OH)4, (OH)3Si-O-Si-(OH)3, [SiOn/2(OH)4-n]m) are transported through the plant to a deposition site (the cell wall, the cell lumen and in intercellular and extracellular spaces) where the silica concentration is raised to the extent that it precipitates out to form a solid hydrated silica body ( Figure  16A) [109,114]. The silica bodies, the phytoliths, exhibit interesting morphologies as illustrated in Figure 16B. Although amorphous silica has only short-range order, cellulose and other carbohydrates are ordered structures, and therefore impart a certain shape on the silica that is deposited [3].  [115] and image B is reproduced from [116], both with permission from John Wiley and Sons.
One of the proposed roles of silica in plants is to crosslink their cell wall-forming polymers, and thereby increasing their compressive strength [117]. Silicification is preferentially chosen in certain species for improving mechanical properties of some tissues. For improving mechanical properties, these plants could technically 'choose' between inorganic SiO2 fortification, and organic lignin fortification. While silicification comes at lower metabolic cost than lignin formation, the water repellency of SiO2 cannot compare to that of lignin, and thus an optimal property compromise is generated by a composite of both [111]. Among other functions, it has been suggested that phytoliths serve a variety of purposes, including (i) to keep the leaf blades erect, thus allowing light to reach the lower leaves and hence increasing the extent of photosynthesis; (ii) to protect from UV radiation; (iii) to promote structural rigidity, i.e., preventing it from falling over and giving mechanical strength and rigidity to leaves; and (iv) to act as a defense against both vertebrate and invertebrate herbivores by Scale bar = 10 mm. Image A is reproduced from [115] and image B is reproduced from [116], both with permission from John Wiley and Sons.
One of the proposed roles of silica in plants is to crosslink their cell wall-forming polymers, and thereby increasing their compressive strength [117]. Silicification is preferentially chosen in certain species for improving mechanical properties of some tissues. For improving mechanical properties, these plants could technically 'choose' between inorganic SiO 2 fortification, and organic lignin fortification. While silicification comes at lower metabolic cost than lignin formation, the water repellency of SiO 2 cannot compare to that of lignin, and thus an optimal property compromise is generated by a composite of both [111]. Among other functions, it has been suggested that phytoliths serve a variety of purposes, including (i) to keep the leaf blades erect, thus allowing light to reach the lower leaves and hence increasing the extent of photosynthesis; (ii) to protect from UV radiation; (iii) to promote structural rigidity, i.e., preventing it from falling over and giving mechanical strength and rigidity to leaves; and (iv) to act as a defense against both vertebrate and invertebrate herbivores by increasing the abrasiveness of grass leaves [3,114,[118][119][120]. Note that different phytolith types present in various plant species have been compiled in a recent review by Sharma and coworkers [121].
Silicified structures are also largely found in grasses grown for their edible grains, such as cereals (e.g., rice, oat and wheat) [114,122]. Rice, for example, is the plant accumulating the highest known amounts of silicon. Silicon is most abundant as cuticle-silica layer in the inflorescence husk [12,123].
Cuticle-silica has important roles as a component for enhancing mechanical properties, stability, and as a physical barrier [124]. It was shown for seedlings of soybeans, wheat, and reed, that an amorphous silica double layer near the epidermis reduces stress induced by UV-radiation, acting like a glassy barrier and reducing the UV transmission ( Figure 17) [119].
increasing the abrasiveness of grass leaves [3,114,[118][119][120]. Note that different phytolith types present in various plant species have been compiled in a recent review by Sharma and coworkers [121].
Silicified structures are also largely found in grasses grown for their edible grains, such as cereals (e.g., rice, oat and wheat) [114,122]. Rice, for example, is the plant accumulating the highest known amounts of silicon. Silicon is most abundant as cuticle-silica layer in the inflorescence husk [12,123]. Cuticle-silica has important roles as a component for enhancing mechanical properties, stability, and as a physical barrier [124]. It was shown for seedlings of soybeans, wheat, and reed, that an amorphous silica double layer near the epidermis reduces stress induced by UV-radiation, acting like a glassy barrier and reducing the UV transmission ( Figure 17) [119]. The hardness and stiffness of bamboo ( Figure 18A) is due to the presence of intracellular silica in the fiber structure. Some species of bamboo contain extracellular silica in the hollow stems as a gelatinous mass known as 'tabashir'. It can be isolated from the plant tissues and appears to be the residue of the watery liquid also found in the hollow internodes of the plant. Once the bamboo ages and the gelatinous mass become solid, it deposits in the pit cavity as loose grains ( Figure 18B). The reason for the origin of such enormous amounts of silica remains to date still unclear. Sanders et al. [125] were the first to study these structures in detail and showed that the tabashir particles ( Figure  18C) were nearly spherical amorphous silica particles of ~100 Å, that give tabashir a milky appearance.  The hardness and stiffness of bamboo ( Figure 18A) is due to the presence of intracellular silica in the fiber structure. Some species of bamboo contain extracellular silica in the hollow stems as a gelatinous mass known as 'tabashir'. It can be isolated from the plant tissues and appears to be the residue of the watery liquid also found in the hollow internodes of the plant. Once the bamboo ages and the gelatinous mass become solid, it deposits in the pit cavity as loose grains ( Figure 18B). The reason for the origin of such enormous amounts of silica remains to date still unclear. Sanders et al. [125] were the first to study these structures in detail and showed that the tabashir particles ( Figure 18C) were nearly spherical amorphous silica particles of~100 Å, that give tabashir a milky appearance.
increasing the abrasiveness of grass leaves [3,114,[118][119][120]. Note that different phytolith types present in various plant species have been compiled in a recent review by Sharma and coworkers [121].
Silicified structures are also largely found in grasses grown for their edible grains, such as cereals (e.g., rice, oat and wheat) [114,122]. Rice, for example, is the plant accumulating the highest known amounts of silicon. Silicon is most abundant as cuticle-silica layer in the inflorescence husk [12,123]. Cuticle-silica has important roles as a component for enhancing mechanical properties, stability, and as a physical barrier [124]. It was shown for seedlings of soybeans, wheat, and reed, that an amorphous silica double layer near the epidermis reduces stress induced by UV-radiation, acting like a glassy barrier and reducing the UV transmission ( Figure 17) [119]. The hardness and stiffness of bamboo ( Figure 18A) is due to the presence of intracellular silica in the fiber structure. Some species of bamboo contain extracellular silica in the hollow stems as a gelatinous mass known as 'tabashir'. It can be isolated from the plant tissues and appears to be the residue of the watery liquid also found in the hollow internodes of the plant. Once the bamboo ages and the gelatinous mass become solid, it deposits in the pit cavity as loose grains ( Figure 18B). The reason for the origin of such enormous amounts of silica remains to date still unclear. Sanders et al. [125] were the first to study these structures in detail and showed that the tabashir particles ( Figure  18C) were nearly spherical amorphous silica particles of ~100 Å, that give tabashir a milky appearance.   [126] with permission from Springer Nature. Image D is adapted from [127] with permission from Elsevier.
Silica, isolated from the plant tissues by ashing or by acid digestion, has often been identified as opal-type (i.e., amorphous SiO 2 ) by optical and electron microscopy, and X-ray diffraction techniques. Whether in plants or animals, at the microscopic level, biogenic silica is always considered to be amorphous, showing no order beyond 10 Å, or approximately three Si-O-Si units. Nevertheless, Sterling [128] identified the first examples of crystalline silica-together with amorphous silica-in strawberry leaves and tabashir. In tabashir, the crystalline parts of SiO 2 could be ascribed to low tridymite and α-cristobalite through X-ray diffraction analysis, and to quartz in strawberry leaves. Reasons for the appearance of crystalline forms of SiO 2 in these plants are yet unclear and, to the best of our knowledge, further observations have not been reported.
Silica bodies can also be present for defense, making some plants distasteful to herbivores or give their tissues a prickly texture. Typical examples are cacti that contain barbs, and rose stems with sharp hooks. The hairs that are responsible for the stinging caused by stinging nettles, the so-called trichomes, are made of fine hollow needles of silica [129]. Studies on the mineralization within Urticaceae, a herbaceous plant which has jagged leaves covered with stinging hairs ( Figure 19A) show that SiO 2 is dominant in all stinging hair tips ( Figure 19B) over any other parts of the structure [130]. These hairs are sharp enough to penetrate skin and inject a mixture of inflammatory substances, including, e.g., histamine, acetylcholine and formic acid [131].
Biomimetics 2020, 5, x FOR PEER REVIEW 20 of 39 (D) TEM image of biogenic hydrated SiO2 particles. Images A-C are reproduced from [126] with permission from Springer Nature. Image D is adapted from [127] with permission from Elsevier.
Silica, isolated from the plant tissues by ashing or by acid digestion, has often been identified as opal-type (i.e., amorphous SiO2) by optical and electron microscopy, and X-ray diffraction techniques. Whether in plants or animals, at the microscopic level, biogenic silica is always considered to be amorphous, showing no order beyond 10 Å, or approximately three Si-O-Si units. Nevertheless, Sterling [128] identified the first examples of crystalline silica-together with amorphous silica -in strawberry leaves and tabashir. In tabashir, the crystalline parts of SiO2 could be ascribed to low tridymite and α-cristobalite through X-ray diffraction analysis, and to quartz in strawberry leaves. Reasons for the appearance of crystalline forms of SiO2 in these plants are yet unclear and, to the best of our knowledge, further observations have not been reported.
Silica bodies can also be present for defense, making some plants distasteful to herbivores or give their tissues a prickly texture. Typical examples are cacti that contain barbs, and rose stems with sharp hooks. The hairs that are responsible for the stinging caused by stinging nettles, the so-called trichomes, are made of fine hollow needles of silica [129]. Studies on the mineralization within Urticaceae, a herbaceous plant which has jagged leaves covered with stinging hairs ( Figure 19A) show that SiO2 is dominant in all stinging hair tips ( Figure 19B) over any other parts of the structure [130]. These hairs are sharp enough to penetrate skin and inject a mixture of inflammatory substances, including, e.g., histamine, acetylcholine and formic acid [131]. Very recently, silica structures were identified in pineapples bracts and shells ( Figure 20) [132]. Their shells feature rosette-like microparticles ( Figure 20B) that were identified as biogenic silica, responsible for giving support and mechanical resistance to the shell structure, among supposedly other, yet unexplored, functions. Very recently, silica structures were identified in pineapples bracts and shells ( Figure 20) [132]. Their shells feature rosette-like microparticles ( Figure 20B) that were identified as biogenic silica, responsible for giving support and mechanical resistance to the shell structure, among supposedly other, yet unexplored, functions.

Aluminum Oxide and Germanium Oxide
One might expect that, during the development of a plant, elements other than silicon and oxygen will be incorporated into the structures of phytoliths structures. Indeed, so far 24 different elements were detected in plant phytoliths [133].
As for silicon, aluminum can also be associated with phytoliths of plants. However, the accumulation of aluminum and silicon appear to be mutually exclusive. High silicon accumulators (e.g., rice) take up little aluminum, while aluminum accumulator plants take up little silicon [134]. Only a very small number of Al-accumulators is known to date. A small number of woody species

Aluminum Oxide and Germanium Oxide
One might expect that, during the development of a plant, elements other than silicon and oxygen will be incorporated into the structures of phytoliths structures. Indeed, so far 24 different elements were detected in plant phytoliths [133].
As for silicon, aluminum can also be associated with phytoliths of plants. However, the accumulation of aluminum and silicon appear to be mutually exclusive. High silicon accumulators (e.g., rice) take up little aluminum, while aluminum accumulator plants take up little silicon [134]. Only a very small number of Al-accumulators is known to date. A small number of woody species (e.g., conifers) accumulate aluminum in the form of aluminosilicates in their phytolith structures [135]. Although aluminum is an abundant element, it is not essential for biological systems and their processes. The abundance of aluminum (~8% in the crust compared to~27% for Si) and the inexistence of a biological system associated with it are intriguing. One possible explanation is that most of Al released by the weathering of aluminosilicates present in the soil is actually taken up geologically, to form phyllosilicates. The higher the Si concentration in soil, the more Al-phyllosilicates form over aluminum oxides. Furthermore, the complexation of Al 3+ by organic matter prevents aluminum oxide precipitation [9,136].
Another M x O y that one might expect to find in organisms is germanium oxide (germania) due to its chemical similarity with silica (yet at low abundance in the crust: 0.00014%). Trace quantities of Ge can be found within the silica structures made by diatoms or sponges; however, GeO 2 cannot be found as part of any living structure. In fact, elevated concentrations of germanic acid have been observed to poison diatoms and sponges, and to produce distortions in the silica structures formed by these organisms [137].

Iron Oxides
Iron oxides are found in organisms to accumulate iron for future metabolic needs, serving for strengthening and hardening of tissues, intracellular iron storage, detoxification, and sensing of magnetic fields [33]. Examples of biogenic iron oxides are found in bacteria, algae, bees, mollusks, fish, pigeons and mammals [138].
Ferrihydrite (5Fe 2 O 3 ·9H 2 O), lepidocrocite (γ-FeOOH), goethite (α-FeOOH) and ferric oxide (Fe 2 O 3 ·nH 2 O) have been found in animal species. The major iron oxide present in living nature is however magnetite (Fe 3 O 4 ), which is ferrimagnetic and has a hardness of 6.5 on the Mohs scale [33]. The first discovery of magnetic Fe 3 O 4 in biological systems was in the teeth (denticles) of chiton mollusks, a species of marine mollusks from the kingdom animalia and phylum mollusca ( Figure 21A,B) [68]. The high iron concentration in chiton denticles allows them to abrade particles of algae from the substrate they live on, which they ingest [139].
It was shown that the mineralization processes of the teeth in Cryptochiton stelleri, a specimen of chiton, features the precipitation of iron minerals inside an organic matrix ( Figure 21C). As the teeth mature, the ferric mineral ferrihydrite is transformed to magnetite (Fe 3 O 4 ) [140]. Recently, it was hypothesized that the synthesis of magnetite in chiton teeth occurs through the following procedure ( Figure 21C): Initially, soluble ferric ions are transported into the tooth matrix, made of α-chitin and proteins (e.g., ferritin), through the tooth surface (step 1). The adsorbed hydrated iron species precipitate as ferrihydrite with the aid of ferritin proteins (step 2). Then, ferrihydrite is converted to magnetite via a solid-state transformation and magnetite crystals grow along the chitin fiber until the space between particles and chitin fibers is completely filled (step 3). In the end, the tooth core region of apatite (Ca 5 (PO 4 ) 3 (OH,F,Cl)) or iron phosphate mineralizes to complete the tooth formation (step 4). This mechanistic hypothesis was based on a combination of structural analysis and proteomics [141].
precipitate as ferrihydrite with the aid of ferritin proteins (step 2). Then, ferrihydrite is converted to magnetite via a solid-state transformation and magnetite crystals grow along the chitin fiber until the space between particles and chitin fibers is completely filled (step 3). In the end, the tooth core region of apatite (Ca5(PO4)3(OH,F,Cl)) or iron phosphate mineralizes to complete the tooth formation (step 4). This mechanistic hypothesis was based on a combination of structural analysis and proteomics [141]. Step 1: Organic tooth matrix around the unmineralized tooth core, which adsorbed Fe 3+ ; Step 2: Fe 3+ is first transformed into ferrihydrite; Step 3: conversion of ferrihydrite into magnetite; Step 4: mineralization of magnetite shell proceeds and the tooth core is also mineralized to phosphates. Image A reproduced from [142] by Brooker and Shaw, 2012, reproduced under the terms of the Creative Commons Attribution 3.0 License. Image B is reproduced from [141] with permission from Springer Nature.
After the initial discovery of biogenic magnetic iron oxide in the teeth of chitons by Lowenstam in the 1970s [140], certain bacteria were discovered to contain chains of single crystalline magnetite particles that act as small magnets and allow for these bacteria to align along the magnetic field of the Earth [45]. The iron oxide bearing bacteria are named 'magnetotactic bacteria'. In these, uniformly sized particles of magnetite are often arranged in different chains and their morphologies include rods, vibrios, spirilla, cocci, and ovoid bacteria ( Figure 22). Nothe the following definition: Vibrio: a genus of Gram-negative bacteria, possessing a curved-rod (comma) shape. Spirilla: Gram-negative bacteria with a helical or spiral shape. Cocci: any bacterium that has a spherical shape. Magnetotactic Step 1: Organic tooth matrix around the unmineralized tooth core, which adsorbed Fe 3+ ; Step 2: Fe 3+ is first transformed into ferrihydrite; Step 3: conversion of ferrihydrite into magnetite; Step 4: mineralization of magnetite shell proceeds and the tooth core is also mineralized to phosphates. Image A reproduced from [142] by Brooker and Shaw, 2012, reproduced under the terms of the Creative Commons Attribution 3.0 License. Image B is reproduced from [141] with permission from Springer Nature.
After the initial discovery of biogenic magnetic iron oxide in the teeth of chitons by Lowenstam in the 1970s [140], certain bacteria were discovered to contain chains of single crystalline magnetite particles that act as small magnets and allow for these bacteria to align along the magnetic field of the Earth [45]. The iron oxide bearing bacteria are named 'magnetotactic bacteria'. In these, uniformly sized particles of magnetite are often arranged in different chains and their morphologies include rods, vibrios, spirilla, cocci, and ovoid bacteria ( Figure 22). Nothe the following definition: Vibrio: a genus of Gram-negative bacteria, possessing a curved-rod (comma) shape. Spirilla: Gram-negative bacteria with a helical or spiral shape. Cocci: any bacterium that has a spherical shape. Magnetotactic bacteria are the most intensely studied types of biogenic iron oxides. A list with all the isolated and characterized species of magnetotactic bacteria is reported in [143]. Blakemore was the first to describe the presence of iron-rich particles within membrane vesicles [45]. In these systems, the particles are enclosed in membrane vesicles, forming structures known as a magnetosomes and enabling the organism with a behavior known as magnetotaxis (the property of movement along magnetic fields) [144].
The mineralization of magnetic particles in magnetotactic bacteria is still under investigation. Based on Mössbauer spectroscopy and biochemical analyses, it was suggested that for bacterial magnetite formation, Fe 3+ ions are taken up from the environment and reduced intracellularly. Then, mineral precipitation occurs within the magnetosome vesicles, possibly by a partial reduction in hydrated ferric oxide [145][146][147].
Using a combination of Mössbauer spectroscopy and electron microscopy, Schuler et al. examined the cellular iron uptake in magnetotactic bacteria in detail, and hypothesized the following mechanism of formation of biogenic Fe 3 O 4 ( Figure 23): First, the bacteria take up either ferric iron (Fe 3+ ) or ferrous iron (Fe 2+ ) (Step 1) and convert it intracellularly to a ferrous high-spin species (Step 2). These iron species remain associated with the cytoplasmic membrane until mineralization (Step 3), when the magnetite crystals ( Figure 23F) grow to entirely fill the magnetosome compartment (Step 4) [148].
Their analysis indicated that ferritin might play an important role in the coprecipitation of ferric and ferrous iron ions at the magnetosome membrane, although its exact role has not been fully elucidated. Ferritin is a hollow spherical protein bearing iron ions in its cavity ( Figure 23E). The iron core of the protein is described as a mineral of the ferrihydrite type, and it is considered essential for the iron storage of various organisms, including humans [149]. Ferritin is commonly considered a crucial precursor in the synthesis of magnetite in diverse biological systems [150].
Biomimetics 2020, 5, x FOR PEER REVIEW 23 of 39 bacteria are the most intensely studied types of biogenic iron oxides. A list with all the isolated and characterized species of magnetotactic bacteria is reported in [143]. Blakemore was the first to describe the presence of iron-rich particles within membrane vesicles [45]. In these systems, the particles are enclosed in membrane vesicles, forming structures known as a magnetosomes and enabling the organism with a behavior known as magnetotaxis (the property of movement along magnetic fields) [144]. The mineralization of magnetic particles in magnetotactic bacteria is still under investigation. Based on Mössbauer spectroscopy and biochemical analyses, it was suggested that for bacterial magnetite formation, Fe 3+ ions are taken up from the environment and reduced intracellularly. Then, mineral precipitation occurs within the magnetosome vesicles, possibly by a partial reduction in hydrated ferric oxide [145][146][147].
Using a combination of Mössbauer spectroscopy and electron microscopy, Schuler et al. examined the cellular iron uptake in magnetotactic bacteria in detail, and hypothesized the following mechanism of formation of biogenic Fe3O4 ( Figure 23): First, the bacteria take up either ferric iron (Fe 3+ ) or ferrous iron (Fe 2+ ) (Step 1) and convert it intracellularly to a ferrous high-spin species (Step 2). These iron species remain associated with the cytoplasmic membrane until mineralization (Step 3), when the magnetite crystals ( Figure 23F) grow to entirely fill the magnetosome compartment (Step 4) [148]. Their analysis indicated that ferritin might play an important role in the coprecipitation of ferric and ferrous iron ions at the magnetosome membrane, although its exact role has not been fully elucidated. Ferritin is a hollow spherical protein bearing iron ions in its cavity ( Figure 23E). The iron core of the protein is described as a mineral of the ferrihydrite type, and it is considered essential for the iron storage of various organisms, including humans [149]. Ferritin is commonly considered a crucial precursor in the synthesis of magnetite in diverse biological systems [150]. The discovery of the existence of inorganic magnetic materials in bacteria prompted investigations of their existence and role in the orientation of higher animals. It was observed that some migratory animals appear to be sensitive to magnetic fields. With further studies, the occurrence of magnetic particles was reported in different tissues of several animals, e.g., rodents [152], bats [153], honeybees [2], pigeons [154,155], fishes [156], and marine mammals [157]. Even in humans, magnetic iron oxide nanoparticles have been identified in different tissues from the brain, heart, liver, and spleen, and it is deemed possible that they are of biogenic origin [158][159][160][161].
The size and morphology of the magnetite particles are species-specific ( Figure 24). Biogenic The discovery of the existence of inorganic magnetic materials in bacteria prompted investigations of their existence and role in the orientation of higher animals. It was observed that some migratory animals appear to be sensitive to magnetic fields. With further studies, the occurrence of magnetic particles was reported in different tissues of several animals, e.g., rodents [152], bats [153], honeybees [2], pigeons [154,155], fishes [156], and marine mammals [157]. Even in humans, magnetic iron oxide nanoparticles have been identified in different tissues from the brain, heart, liver, and spleen, and it is deemed possible that they are of biogenic origin [158][159][160][161].
The size and morphology of the magnetite particles are species-specific ( Figure 24). Biogenic magnetite particles can be classified according to their size and magnetic properties into: (i) large particles (>1.0 µm) with their magnetic moments largely canceling each other out (known as multi domains); (ii) particles in the range between about 0.05-1.0 µm featuring a stable magnetic moment, and acting as tiny permanent magnets (known as single domain); and (iii) superparamagnetic particles (3-5 nm), with magnetic moments that can be relatively easily aligned by an external magnetic field [162,163]. It is assumed that the magnetic crystal sizes are determined by spatial constraints exerted by the local environment (such as the magnetosome vesicle size). Furthermore, the biomineralization of the ferrihydrite core of ferritin is considered a possible pathway for the formation of larger magnetite particles [150]. Thus, growth of Fe 3 O 4 particles in living systems might be regulated to generate the species-specific sizes that are effective for the distinct purpose of the species. One of the limitations in these studies relies on the magnetite nanoparticles' sizes: given that iron is common in several physiological processes, is extremely difficult (with the current analytical tools) to differentiate between magnetic particles and the iron compounds used in other metabolic activities [164].

Manganese Oxides
Manganese oxides (including oxides, hydroxides, and oxyhydroxides) are important minerals in biogeochemical cycles. The oxidation of soluble Mn 2+ species to insoluble Mn 3+/4+ oxides is an environmentally important process since MnO2 can oxidize a variety of organic and inorganic compounds, scavenge many metals from the environment (e.g., Cu, Co, Cd, Zn, Ni, and Pb), and Figure 24. Magnetite in living systems subdivided as a function of particle size and magnetic behavior (single domain, multi domain or superparamagnetic). Adapted from [163] with permission from Springer Nature. Information on additional species was compiled from [164].

Manganese Oxides
Manganese oxides (including oxides, hydroxides, and oxyhydroxides) are important minerals in biogeochemical cycles. The oxidation of soluble Mn 2+ species to insoluble Mn 3+/4+ oxides is an environmentally important process since MnO 2 can oxidize a variety of organic and inorganic compounds, scavenge many metals from the environment (e.g., Cu, Co, Cd, Zn, Ni, and Pb), and serve as electron acceptor for anaerobic (Anaerobic respiration is the respiration using electron acceptors other than O 2 )respiration of certain living organisms [165].
In the environment, the catalytic role is filled by a class of microorganisms referred to as 'manganese oxidizers'. To date, the only species bearing biogenic Mn oxides are Mn-oxidizing/reducing bacteria and fungi [166], and the involved Mn oxide formation process is largely unresolved. Through laboratory culture experiments, it has been proposed that Mn oxidation and reduction is mainly mediated by bacteria. Over the years, Mn-oxidizing bacteria have been isolated and identified from a wide variety of environments, including both the oceans and freshwaters, sediments, and hydrothermal vents [21,[166][167][168][169]. The mechanism of Mn 2+ oxidation and oxide formation by microorganisms is not well established, however, several studies evidence that certain enzymes (multicopper oxidases), appear to be involved in Mn oxidation in all of these organisms [170][171][172][173].
Manganese oxidizing bacteria species are reported to produce mixed-valence Mn oxides with structures corresponding to the minerals todorokite or birnessite [174][175][176][177]. The todorokite-type tunnel and birnessite-type layered structures found in biogenic manganese oxides are structurally closely related to each other. Synthetically speaking, birnessite can be transformed easily into todorokite via hydrothermal treatment and cation exchange [178,179].
Despite bacteria being the dominant Mn-oxidizing organisms, Mn-oxidizing fungi have also been observed in extreme environments such as deep-sea ferro-manganese crusts [180], and in terrestrial environments [181,182]. In some surface and terrestrial environments, fungal Mn oxidation is more important than bacterial oxidation [183]. Despite the lack of a universally accepted model, some experimental work tries to expand the knowledge on biogenic Mn x O y in diverse species of Mn-oxidizing fungi by characterizing them through microscopic and spectroscopic techniques [182,184,185]. The studies reveal that, depending on the species of Mn-oxidizing fungi, different Mn x O y sizes and morphologies, and chemical structures are found ( Figure 25). For example, the Mn oxides produced by Plectosphaerella cucumerina type ( Figure 25A-C) have a typical nanoparticulate, plate-like morphology, as the ones observed for Mn(II)-oxidizing bacteria. Mn oxides observed in Stagonospora sp. type ( Figure 25D-F) form densely packed filaments of Mn oxides. The third example, the Acremonium strictum ( Figure 25G-I) exhibits rather poorly defined morphologies and the Mn oxide conglomerate presents a honeycomb-like appearance [185].
Petkvok et al. showed that Mn-oxidizing fungi prefer a less moist environment, oxidize Mn ions relatively slowly, and are prone to produce todorokite particles of higher crystallinity (almost defect-free), compared to Mn-oxidizing bacteria [184]. Santelli et al. have shown that the fungal organic matrices play an important role in organizing Mn x O y structures in order to decrease thermodynamic barriers for precipitation of more crystalline phases like todorokite [185].
Mn oxides precipitated by the Mn-oxidizing organisms accumulate on the extracellular matrix of the organisms for both bacteria and fungi. However, to date, the physiological reasons behind the Mn oxidation is yet unclear. Some authors suggest that one of the reasons might be to harvest energy for their growth [13,166]. Further hypotheses are that the resulting Mn x O y can increase the accessibility of organic nutrients and protect the microorganism from potentially toxic compounds, reactive oxygen species and UV radiation stress [186,187]. Zerfaß et al. have recently shown that the Mn oxides in Roseobacter sp. strain AzwK-3b, are involved in the catalysis of nitrites (known as bacteria inhibitors) into nontoxic nitrate compounds, which thus protects bacteria against nitrite [188].
Although biogenic Mn x O y are only produced by simple organisms such as bacteria and fungi, it has been found that they play a role in the symbiosis with more complex living systems. For example, certain plants bear Mn-oxidizing bacteria or fungi within their tissues. Here, the microorganisms support the plant growth and development. Recent studies on wetland plant species (e.g., Egeria densa or Suaeda salsa pall) have revealed that their associated bacteria have Mn-oxidizing activities, enabling the synthesis of Mn x O y biofilms on the plant roots' surfaces [189][190][191]. The appearance of Mn oxides as plaques on the surface and in the pit (a tissue in the stems of vascular plants, which store and transport nutrients throughout the plant) of these wetland plants enhance further precipitation of Mn oxides on the plant roots, possibly serving as an oxidant of heavy metals and pollutants and as a scavenger of trace nutrients to sustain the growth of these plants in saline and heavy metal-contaminated wetlands.
oxidizing fungi by characterizing them through microscopic and spectroscopic techniques [182,184,185]. The studies reveal that, depending on the species of Mn-oxidizing fungi, different MnxOy sizes and morphologies, and chemical structures are found ( Figure 25). For example, the Mn oxides produced by Plectosphaerella cucumerina type ( Figure 25A-C) have a typical nanoparticulate, plate-like morphology, as the ones observed for Mn(II)-oxidizing bacteria. Mn oxides observed in Stagonospora sp. type ( Figure 25D-F) form densely packed filaments of Mn oxides. The third example, the Acremonium strictum ( Figure 25G-I) exhibits rather poorly defined morphologies and the Mn oxide conglomerate presents a honeycomb-like appearance [185].
Petkvok et al. showed that Mn-oxidizing fungi prefer a less moist environment, oxidize Mn ions relatively slowly, and are prone to produce todorokite particles of higher crystallinity (almost defectfree), compared to Mn-oxidizing bacteria [184]. Santelli et al. have shown that the fungal organic matrices play an important role in organizing MnxOy structures in order to decrease thermodynamic barriers for precipitation of more crystalline phases like todorokite [185].

Biomimetics of Biogenic Metal Oxide Structures and Further Inspirations and Perspectives for Materials Synthesis
Hierarchical and functional inorganic M x O y structures are found in living organisms of all the kingdoms, from simple bacteria or fungi to more complex plants and animals. Clearly, these structures present an intriguing source of inspiration for novel synthetic pathways for the production of materials, but also for novel synthetic materials.
One approach in the biomimicry of biogenic M x O y is to investigate the biomolecules that organisms use for controlling M x O y precipitation for synthetic M x O y generation, as well as to derive synthetic variants of these biomolecules. This includes to extract, isolate, characterize, and understand the role of biomolecules involved in the mineralization. To date, several examples of successful in vitro mineralization employing proteins and peptides extracted from organisms that biosynthesize M x O y have been reported. As several reviews have summarized both the biomimetics of natural M x O y assemblies [14,15,[192][193][194], and biomimetics approaches to magnetic materials [195], we will not go into further detail here.
Biomolecules mediating biogenic M x O y formation have also been utilized to synthesize materials beyond those produced by the original living organism. For instance, current approaches include the in vitro use of proteins from diatoms (so-called silaffins) [196], or silicatein filaments from sponges [197], to obtain TiO 2 nanostructures (Figure 26). It is shown that both types of proteins, although from different species, are capable of catalyzing and templating the hydrolysis and condensation of titanium alkoxides to form TiO 2 . Most interestingly, TiO 2 obtained from silaffin-mediated synthesis generates spherical, diatom-esque morphologies. Furthermore, proteins and peptides extracted from diatoms were used in the in vitro mineralization of new amorphous silica structures [198], and gallium oxide [199]. In addition, other proteins have been used to generate M x O y that are not found in living organisms, such as germanium oxide [200], cobalt oxide [201], zinc oxide [202], multi component oxides [203], and perovskite-type oxides [204].   [197] with permission from American Chemical Society. Images in B are adapted from [196] with permission from John Wiley and Sons.
Aside biomimicry of biological MxOy synthesis, biogenic MxOy can also serve as inspiration for inorganic-organic composites and hybrids. Note that the term 'composite' was historically used for larger structures not featuring strong bonding between matrix and dispersed phase, while 'hybrid' was reserved for strongly bonded inorganic-organic materials with phase domains in colloidal size range (1-1000 nm). Nowadays, both terms are often used interchangeably. A first learning that one can draw from biogenic MxOy-which, with the exception of Fe oxides, are composites of FexOy intricately connected to biomolecules-is which types of organic compounds MxOy are likely (as observed in nature) to be compatible with. The interfaces between inorganic and organic phases in composites/hybrids are both the loci that have the strongest impact on synergistic properties and also the loci of materials failure [205]. From the distinct combinations of MxOy with, e.g., certain polysaccharides or peptides and proteins in biogenic MxOy materials, one can infer with high certainty that a combination of closely related materials will also exhibit good compatibility. Indeed, the recent developments in the field of cross-linked metaloxides particles uses polysaccharides crosslinkers such as alginate [206]. Several examples of so-called 'extreme biomimetic' synthesis have exploited the generation of MxOy-polysaccharide composites by extremophile organisms [6], to generate, e.g., chitin/SiO2 [207], chitin/ZnO [208], and chitin/ZrO2 [209]. Furthermore, biogenic MxOy in living organisms are never (as from all reported examples to date) biosynthesized concomitantly with the biomolecules one finds in the final MxOy composites. This allows for the conclusion that the truly simultaneous synthesis of organic and inorganic components is likely to yield radically different synthetic hybrid materials than what is found in nature. Indeed, rare examples of truly concomitant synthesis yield fascinating materials structures and properties, e.g., with respect to crystallinity [210]. Alternatively, one might also conclude that the intricate MxOy composites found in nature cannot be synthetically generated through simultaneous synthesis, but actually require the presence of biomolecules (with, e.g., the templating and structure-directing effects), before MxOy is precipitated.
Instead of gathering inspiration from the actual materials found in biominerals, one might also look at the types of reactions that lead to them in living organisms, and apply them to chemically  [197] with permission from American Chemical Society. Images in B are adapted from [196] with permission from John Wiley and Sons.
The use of compounds of biological origin extracted from organisms for materials synthesis has, however, some drawbacks. The species may be difficult to obtain, many require specialized facilities for their growth, and they yield limited quantities of the desired biomolecules. Furthermore, the number of biomineralization proteins that have been identified (and sequenced) to date is still quite limited.
Aside biomimicry of biological M x O y synthesis, biogenic M x O y can also serve as inspiration for inorganic-organic composites and hybrids. Note that the term 'composite' was historically used for larger structures not featuring strong bonding between matrix and dispersed phase, while 'hybrid' was reserved for strongly bonded inorganic-organic materials with phase domains in colloidal size range (1-1000 nm). Nowadays, both terms are often used interchangeably. A first learning that one can draw from biogenic M x O y -which, with the exception of Fe oxides, are composites of Fe x O y intricately connected to biomolecules-is which types of organic compounds M x O y are likely (as observed in nature) to be compatible with. The interfaces between inorganic and organic phases in composites/hybrids are both the loci that have the strongest impact on synergistic properties and also the loci of materials failure [205]. From the distinct combinations of M x O y with, e.g., certain polysaccharides or peptides and proteins in biogenic M x O y materials, one can infer with high certainty that a combination of closely related materials will also exhibit good compatibility. Indeed, the recent developments in the field of cross-linked metaloxides particles uses polysaccharides cross-linkers such as alginate [206]. Several examples of so-called 'extreme biomimetic' synthesis have exploited the generation of M x O y -polysaccharide composites by extremophile organisms [6], to generate, e.g., chitin/SiO 2 [207], chitin/ZnO [208], and chitin/ZrO 2 [209]. Furthermore, biogenic M x O y in living organisms are never (as from all reported examples to date) biosynthesized concomitantly with the biomolecules one finds in the final M x O y composites. This allows for the conclusion that the truly simultaneous synthesis of organic and inorganic components is likely to yield radically different synthetic hybrid materials than what is found in nature. Indeed, rare examples of truly concomitant synthesis yield fascinating materials structures and properties, e.g., with respect to crystallinity [210]. Alternatively, one might also conclude that the intricate M x O y composites found in nature cannot be synthetically generated through simultaneous synthesis, but actually require the presence of biomolecules (with, e.g., the templating and structure-directing effects), before M x O y is precipitated.
Instead of gathering inspiration from the actual materials found in biominerals, one might also look at the types of reactions that lead to them in living organisms, and apply them to chemically quite different compounds that, however, form by similar mechanisms. We have recently explored such strategies that are however inspired by materials formation in non-living natural systems, i.e., so-called 'geomimetics' [6]. Prompted through the fact that metal oxides, such as the here intensively discussed SiO 2 , but also various silicates and all natural zeolites, are in the Earth's crust forming through polycondensation (i.e., the addition of small molecules or ions to one another accompanied by the release of one or several H 2 O molecules at each addition step) under hydrothermal conditions (i.e., in liquid H 2 O at T > 100 • C and p > 1 bar), we have explored the formation of organic molecules under hydrothermal conditions [211]. Through geomimetic hydrothermal syntheses, several types of compounds (even highly aromatic) could to date be generated, including polyimides [212][213][214][215][216], low-molecular weight imide and imidazole dyes [217,218], polybenzimidazoles and pyrrone polymers [219], and even simultaneously synthesized polyimide-SiO 2 hybrid materials [210]. In analogy, it is conceivable that the fact that M x O y are formed in living organisms under a given species-specific set of formation conditions (aqueous environment, moderate temperatures, a certain pH range, the presence of certain additives), allows for synthesizing organic materials that mechanistically form by closely related reactions (again, e.g., condensations) under similar conditions. Finally, especially in times of increasing awareness of the scarceness of natural resources and several other aspects of sustainability, biogenic M x O y can actually be used as resources. For instance, there are several reports on the use of rice rusk (which is with up to 20% hydrated SiO 2 in dry weight highly silicified) as resources for the generation of silsesquioxane building blocks [220], and SiO 2 nanoparticles [221,222]. Along these lines, it is also conceivable to generate advanced materials through the pyrolysis of biogenic M x O y . Similar approaches have been reported for heavy metal nanoparticles supported on carbon materials through the pyrolysis of thale cress plants grown on Pd-enriched soils. Clark and coworkers could generate carbon-supported Pd 0 -nanoparticles and show the effectiveness of these materials as catalysts [223].

Conclusions
With this review, we have provided an overview of the metal oxides (SiO 2 , iron and manganese oxides) found in the five kingdoms of living nature. It has become clear that there are several functional biogenic M x O y structures, spanning, e.g., from amorphous to crystalline, presenting magnetic and/or oxidative properties, that can be generated biologically. To date, for all known biogenic M x O y , we have summarized the current understanding of (i) where their precursors come from, (ii) how the precursors are taken up by the organisms, (iii) how the resulting M x O y are precipitated, and (iv) which structures for which purposes result. Examples of biomimetic approaches for M x O y were shown to demonstrate the ongoing efforts in biomineralization research. Metal oxides in living nature are incredibly complex and understanding their architectural design principles can still provide a large body of inspiration for biologists, chemists, and material scientists alike to create a plethora of novel materials.